**Inelastic electron tunneling spectroscopy at local defects in graphene**

J. Fransson,^{1,*}J.-H. She,^{2}L. Pietronero,^{3,4}and A. V. Balatsky^{2,5,6}

1*Department of Physics and Astronomy, Uppsala University, Box 516, SE-751 21 Uppsala, Sweden*

2*Theoretical Division, Los Alamos National Laboratory, Los Alamos, New Mexico 87545, USA*

3*Dipartimento di Fisica, La Sapienza Universita di Roma, Piazalle A. Moro 5, 00185, Rome, Italy*

4*CNR-ISC, Via dei Taurini 19, 00185, Rome, Italy*

5*Center Integrated Nanotechnology, Los Alamos National Laboratory, Los Alamos, New Mexico 87545, USA*

6*NORDITA, Roslagstullsbacken 23, SE-106 91 Stockholm, Sweden*

(Received 15 December 2012; revised manuscript received 20 March 2013; published 3 June 2013)
We address local inelastic scattering from the vibrational impurity adsorbed onto graphene and the evolution
of the local density of electron states near the impurity from a weak to strong coupling regime. For weak coupling
the local electronic structure is distorted by inelastic scattering developing peaks or dips and steps. These features
*should be detectable in the inelastic electron tunneling spectroscopy d*^{2}*I /dV*^{2}using local probing techniques.

Inelastic Friedel oscillations distort the spectral density at energies close to the inelastic mode. In the strong
*coupling limit, a local negative U center forms in the atoms surrounding the impurity site. For those atoms, the*
Dirac cone structure is fully destroyed, that is, the linear energy dispersion as well as the V-shaped local density
*of electron states is completely destroyed. We further consider the effects of the negative U formation and its*
*evolution from weak to strong coupling. The negative U site effectively acts as a local impurity such that sharp*
resonances appear in the local electronic structure. The main resonances are caused by elastic scattering off the
impurity site, and the features are dressed by the presence of vibrationally activated side resonances. Going from
weak to strong coupling, changes the local electronic structure from being Dirac-cone-like including midgap
states, to a fully destroyed Dirac cone with only the impurity resonances remaining.

DOI:10.1103/PhysRevB.87.245404 *PACS number(s): 73.40.Gk, 73.43.Fj, 03.65.Yz, 68.49.Df*

**I. INTRODUCTION**

Graphene has been at the center of attention ever since
its was first synthesized and studied for its unique physical
properties.^{1–5}While its properties are interesting on their own,
an increasing effort is also being directed towards modifica-
tions of graphene. The functionalization of graphene has been
achieved by depositing H atoms, thus, creating graphane,^{6}
which is an insulator with a band gap of the order of 3–6 eV.

Chemical acid treatment may lead to vacancy formation in
graphene,^{7} which tends to increase its conductivity due to a
metallic-like density of electron states (DOS) in the vicinity
of the vacancies.^{8}The role of single and double vacancies in
graphene has also been theoretically investigated, showing the
emergence of midgap states.^{9}

Modifications of electronic states and of the excitation
spectrum of a given material is crucial for a more efficient
functionalization. Examples of spectroscopies that are sensi-
tive to electronic properties are photoemission and photoab-
sorption techniques which give access to the bulk electronic
structure and local scanning techniques such as atomic force
microscopy^{10,11}and scanning tunneling microscopy^{12}(STM).

They are employed for studies of spatial inhomogeneities^{13}
and local spectral properties.^{14}

By studying the response to defects in or on the material im-
portant spectroscopic information can be accessed.^{15}For local
probes this is a particularly fruitful strategy since it is relatively
easy to move the probe on and off the defect. One thus can
achieve comparable measurements of the perturbed and unper-
turbed materials on one and the same sample. Through such an
approach the effects from potential, charge, and magnetic scat-
tering can be measured from both elastic^{16,17} and inelastic^{18}
points of view. Lately is has become routine to measure the
inelastic electron tunneling spectrum (IETS) using STM.

In this paper we apply the same logic to IETS in graphene.

We calculate the local density of electron states (LDOS) for electrons in a tight-binding honeycomb lattice which is used as a model for graphene. The main results are as follows.

(1) In the weak coupling limit and using perturbation theory,
the LDOS near the local vibrational impurity exhibits a kink
*and logarithmic singularity at the vibrational mode ω*_{0}. The
spectral density is significantly modified at energies near the
vibrational mode. We predict those features to be observable
in IETS experiment using local scanning techniques.

(2) For strong coupling, the atoms surrounding the vibra-
*tional impurity forms negative U centers such that the system*
can be considered as a single impurity problem, however, the
impurity is effectively spatially extended. The LDOS is formed
by a series of delta peaks forming a single band at negative
energy. The result is universal in the sense that it is independent
of the band structure of the conduction electrons, see also She
*et al..*^{19}

(3) By coupling the atoms influenced by the vibrational
impurity to the surrounding lattice, we study the evolution of
its LDOS from weak to strong coupling using a many-body
approach. In the weak coupling regime, the Dirac cone is
modified by the introduction of elastic resonances, surrounded
*by inelastic resonances, suggesting that the negative U center*
effectively acts as local impurity. Here the meaning of the
local Dirac cone is related to the local energy dispersion and
LDOS, which deviate from being linear and V-shaped in a
neighborhood of the impurity. In the single impurity case,
we find that all empty, singly, and doubly occupied states
are populated with a finite probability, which suggests the
formation of a local Cooper pair. For increasing coupling, the
set of elastic and inelastic peaks move to lower energies below
the Fermi level, leaving a strongly asymmetric cone structure

around the Fermi level. The Dirac cone is eventually fully destroyed in the strong coupling limit, leaving two resonances which are broadened by the inelastic resonances.

The present work has some similarities and differences
with a previous study of inelastic signatures generated by the
local vibrational defect located on the surface of a topological
insulator^{19} and we point out a few differences which justify
the present study. The first apparent difference is that our
present model for graphene is based on a discrete real-space
lattice instead of a continuum model, which implies that the
exact location of the defect plays a role in the expected
real-space IETS imaging. This assumption also implies that
*the negative U center may be induced at one or more sites*
simultaneously, depending on whether the vibrational defect
couples to one or more C atoms in the graphene lattice. A
second important difference is that we here have to deal with
spinors of pseudospin, in which the entries depend on the
sublattice instead of the electron spin. Thus, here we do not
expect to obtain any possibility for magnetic contrast in the
IETS. Finally, in our present study we treat the evolution from
weak to strong coupling using a different approach by means
of which we verify the main characteristics for each regime
as compared to the case of topological insulators. Using this
approach, however, we capture some central feature of the
many-body (self-energy) aspects induced in the vicinity of the
vibrational defect, and get direct access to the electron number
*of the negative U center. Moreover, due to the discreteness*
and bipartite structure of the graphene lattice, the effective
coupling between C atoms near the vibrational impurity cannot
be removed by canonical transformation, see Sec.IV, which
implies that the electronic and vibrational degrees of freedom
cannot be separated without any (further) approximation.

The paper is organized as follows. First we set up the model for the graphene lattice and the vibrational impurity in Sec.II.

Then we move on to discussing the weak coupling limit using
*a T -matrix approach in Sec.* IIIand the evolution from the
weak to strong coupling limit using a many-body approach in
Sec.IV. We finally conclude the paper in Sec.V.

**II. PROBING THE INELASTIC SCATTERING**
We describe the graphene sheet by the nearest neighbor
interaction model

*H*0 *= −t*

*mnσ*

_{mσ}^{†}*σ**x**nσ**,* (1)

*where the pseudospinor **mσ* *= (a**mσ* *b** _{mσ}*)

*contains the oper-*

^{t}*ators a (b) which annihilate electrons in the A (B) sublattice*

*and where t is the hopping parameter.*

By depositing the molecular defect, e.g., CO, on the graphene sheet, a local vibrational mode can be introduced.

Generically, the molecular vibrations cause nonstatic lattice
distortions. Here we specifically consider the plaquette posi-
tion of the vibrational impurity. An diatomic molecule may,
for example, be located inside a hexagon in a straight up
but slightly tilted position.^{20} The existence of six equivalent
positions that the molecule can assume due to the sixfold
rotational symmetry of the hexagon may cause molecular
rotations, which generate local lattice distortions that can
be described in terms of a local bosonic mode coupling to

TABLE I. Vectors in momentum space connecting the lattice points.

1 2 3

**δ***m* *a(*√

*3,1)/2* *−a(*√

*3,−1)/2* *−a(0,1)*

**δ***Am* *a(0,1)* *−a(*√

*3,1)/2* *a(*√

*3,−1)/2*
**δ***Bm* *−a(*√

*3,−1)/2* *−a(0,1)* *a(*√

*3,1)/2*

the electronic density at the nearest C atoms. Stretching and breathing modes may also be envisioned, especially if the molecule is off-centered within the hexagon. Thus the coupling may be symmetric or asymmetric to the near C atoms. Here we shall consider both possibilities since the later of these can be reduced to effective single and double site interactions.

*We thus introduce ω*0*B*^{†}*B, where B** ^{†}*creates a vibron (local

*bosonic mode) at the energy ω*0, for the local vibrational mode

**at the position R**0. We describe its coupling to the nearest C atoms by

*H*ep=

*mσ*

_{mσ}^{†}**λ(r***m**)**mσ**Q,* (2)
**λ(r***m*)=

*λ**A***(r***m*) 0
0 *λ*_{B}**(r***m*)

*,* (3)

where *λ**A/B***(r***m*)=_{3}

*n*=1*λ**A/Bn**δ(R*0**− r***m***+ δ***A/Bn*) with
**δ***nA/B* are defined in Table I, whereas Q*= B + B** ^{†}* is
the vibrational displacement operator. Here the coupling

*parameters λ*

*n*

*= λ*

*n*

^{}in general. While, in principle, the hopping parameter for the nearest neighbor interaction should be renormalized by the presence of the local vibrations, we neglect this effect here to keep the discussion as simple and transparent as possible.

*Going over to momentum space via, e.g., a**mσ* =
*N*^{−1/2}

**k***a*_{kσ}*e*^{ik}^{·r}^{m}*, where N denotes the number of C atoms*
*in the A sublattice, and analogously for the operators on the B*
sublattice, we can write

*H*0=

**kσ**

*φ(k)a*_{kσ}^{†}*b*_{kσ}*+ H.c.,* (4)
**where the potential φ(k)**= −t_{3}

*m*=1**exp (ik****· δ***m*) such that
*φ(k***+ K**_{±})*≈ ±v**F**k*exp{±i(π/3 − ϕ)}. Here, the vectors δ*m*

are given in Table I, v*F* *= 3at/2, tan ϕ = k**y**/k*_{x}*, and k*=

**|k|, whereas K**_{±}* = ±K = ±2π(*√

*3/3,1)/3a. The electron-*
vibron interaction Hamiltonian is in momentum space written
as

*H*ep=

**kk**^{}*σ*

_{kσ}^{†}**λ(k,k**^{}*)***k***σ**Q,* (5)
where **λ(k,k**^{})*= diag{λ**A***(k,k**^{}*) λ**B***(k,k**^{})} and λ*A/B***(k,k**^{})=

*m**λ**A/B***(r***m*) exp [−i(k − k^{})**· r***m**]/N .*

**III. WEAK COUPLING AND T MATRIX**

We study the effect of the a weak vibrational impurity
*by perturbation theory, which is valid for λ**A/Bn**/t* 1.

**The dressed graphene Green’s function (GF) G(k,k**^{}*; z)*=

**k***|***k**^{†}^{}*(z), suppressing the spin indices, can be calculated*

in terms of the Dyson equation

**G(k,k**^{})**= δ(k − k**^{}**)G**0**(k)+ G**0**(k)**

**κ**

**(k,κ)G(κ,k**^{}*), (6)*

where

**G**0* (k; z)*= 1

*z*

^{2}

**− |φ(k)|**^{2}

*z* *φ(k)*

*φ*^{∗}**(k)** *z*

(7)

is the bare graphene GF, whereas the self-energy is given by

**(k,k**^{}*; z)*=

*mn*

*e*^{−ik·r}^{m}**λ(r***m***)V***mn**(z)λ(r**n**)e*^{ik}^{}^{·r}^{n}*.* (8)
**Here the potential V***mn**(z)= iβ*^{−1}

*ν**D(z**ν***− z)G(r***m***,r***n**; z**ν*),
*where we sum over Bosonic frequencies z**ν* *= i2νπ/β, ν ∈ Z,*
*β* *= 1/k**B**T*, and where we have introduced the local Boson
*GF D(z)= Q|Q(z). In the weak coupling limit, we replace*
*both dressed GFs in by their bare correspondences, using*
*D*_{0}*(z)= 2ω*0*/(z*^{2}*− ω*^{2}_{0}*). Accordingly, the GF is cast in T -*
matrix form in real space

**G(r,r**^{})**= G**0**(r− r**^{})

+

*mn*

**G**_{0}**(r− r***m***)T(r***m***,r**_{n}**)G**_{0}**(r***n***− r**^{}*),* (9a)
**T(r***m***,r*** _{n}*)

**= (δ(r***m*

**− r**

*i*)

**− G**0

**(r**

*m*

**− r**

*i*

**)V**

*ij*

**)**

^{−1}

**V**

*j m*

*,*(9b)

with the bare real-space GF given by

**G**0**(R)**=*2π ω*
*iD*_{c}^{2}

*H*_{0}^{(1)}

*ωR*
*v**F*

*σ*_{0}**cos K****· R − iH**_{1}^{(1)}

*ωR*
*v**F*

*× (σ**x**sin θ**R***sin K****· R + iσ***y**cos θ**R***cos K· R)**

*.*

(10)
*Here H*_{n}^{(1)}*(ω) is the nth Hankel function of the first*
*kind, whereas σ**i**, i= x,y,z, are Pauli matrices and σ*0 is
**the identity matrix. Here also R= r − r**^{}*, θ**R* *= φ**R**+ π/6,*
*tan φ**R* *= (r**y**− r**y*^{}*)/(r**x**− r**x*^{}*), whereas D*_{c}^{2}*= 4πρv**F*^{2}, with sur-
*face density ρ= S/N = k**c*^{2}*/4π (S is the graphene area; k**c*=
2

2√

*3π /3a is the large momentum cutoff).*^{21} We comment
**here that the Fourier transform G**_{0}**(R)**=

**G**_{0}**(k)dk/(2π )**^{2}
is convergent and does not depend on any specific de-
*tails of the large momentum cutoff k**c*, something which
has been discussed by the authors of Ref. 22 for the
case of the Ruderman-Kittel-Kasuya-Yosida (RKKY) inter-
action in graphene and pertains to our discussion as well.

*The cutoff k**c* is introduced to maintain a physical finite
*density ρ.*

Integration around**±K yields the retarded potential (with**
*obvious notation and x**mn***= p|R***mn**|/v**F*)

**V**^{r}_{mn}*(ω)*= 2

*D*_{c}^{2}**λ(r***m*)

*s*=±1

*D** _{c}*
0

1*+ n*0*− f (p)*

*ω− sp − ω*0*+ iδ* + *n*_{0}*+ f (p)*
*ω− sp + ω*0*+ iδ*

* × (J*0

*(x*

*mn*

*)σ*0

**cos K· R**

*mn*

*− isJ*

*n*

*(x*

*mn*

*)[σ*

*x*

*sin θ*

*mn*

**sin K**

**· R + iσ***y*

*cos θ*

*mn*

**cos K**

**· R])pdpλ(r***n*

*).*(11)

*Here, f (x) is the Fermi distribution function whereas n*_{0}=
*n(ω*0*) is the Bose distribution function at ω*0.

We remark here that adatoms may be a source for scattering processes with large momentum transfer which would cause an intervalley coupling. For instance, in mo- mentum space the electron-vibron Hamiltonian has the from

**kk**^{}_{k}^{†}**λ(r) exp[−i(k − k**^{})**· r]****k**^{}, which we can write as

**kp**_{k}^{†}_{+p}**λ(r) exp[−ip · r]****k**. The latter form explicitly in-
**dicates intervalley coupling (large k+ p). However, as we**
*employ the T -matrix expansion, we do not have to worry*
about intervalley coupling since we use the former expression
for the electron-vibron Hamiltonian, in which the momentum
summations are separated hence the valleys are decoupled.

This thus justifies that we integrate around**±K only.**

The electronic structure around the vibrational impurity is
modified at energies near the inelastic mode*±ω*0, where a kink
and peak or dip is created due to the inelastic scattering off
the vibrational center. Using uniform coupling to the hexagon
surrounding the vibrational impurity, in Fig.1(a)we plot the
correction to the local density of electron states (LDOS) and
*its energy derivative (IETS), corresponding to d*^{2}*I /dV*^{2}, and
in Fig.1(b)**at R**_{tip}**− R**0*= a(0,2) for different temperatures.*

The LDOS shows the nontrivial structure at the vibrational

mode which is more apparent in the IETS as it peaks around
*ω*_{0}= 15 meV. Similar features are also predicted for the
*case of IETS signatures in d-wave superconductors*^{24} and in
topological insulators,^{19}as well as for simple metals both for
vibrational^{23}and magnetic imputiry.^{25}

The corresponding real-space mapping of the IETS is
displayed in Fig.1(c)*for energies below, near, and above ω*0.
*For energies below and above ω*0, the presence of the local
vibrations generate low contrast, while the contrast grows
*substantially larger for energies around ω*0. We expect that
the presence of the vibrations generates sufficiently large
*variations in the IETS, i.e., d*^{2}*I /dV*^{2}, to be visible in an
experimental setup.

We complete the weak coupling picture by also plotting
the IETS signatures for asymmetric coupling in Fig. 2,
assuming (a) three, (b) two, and (c) one, C atom being coupled
to the vibrational impurity. As one may expect, the IETS
signal is stronger when more C atoms are coupled to the
vibrational impurity. We also plot different distances between
**the measuring point at r**_{0}**= R**0**+ 2δ***1A* and the atom(s) that
are coupled to the vibrational impurity, clearly showing the
oscillatory behavior that is expected due the inelastic Friedel
oscillations (see the insets of the figure, and Fig.1).

(a)

2 5 8

5 15 25

energy (meV)
δN(**r** **0****,ω****) (x10****−5** **)**

10 K T=100 K 1 K

12
4a_{0}

15 17 20

−2 0 2

IETS

(c)

intensity (arb. units) 0.037 0.040 0.043 0.046

ωN(**r** **0****,**ω**)**

(b)

5 15 25

energy (meV)

FIG. 1. (Color online) (a) Change in the local DOS, corre-
*sponding to dI /dV , and (b) its energy-dependent derivative (IETS),*
*corresponding to d*^{2}*I /dV*^{2}**, at r**0**= R**0**+ 2δ***1A*(star in the inset) in the
*weak coupling limit, for different temperatures T* *= 100, 10, 1 K and*
*vibrational mode ω*0= 15 meV, for uniform coupling to the nearest
C hexagon. (c) Sequence of IETS maps as function of energy, from
*left to right ω= 12, 15, 17, 20 meV, using T = 10 K and spatial*
*broadening = 2a*0*/5. We have added an intrinsic broadening of*
**0.8 meV in the potential V*** _{mn}*.

**IV. EVOLUTION FROM WEAK TO STRONG**
**COUPLING REGIME**

*We here depart from the T -matrix approximation and*
consider the evolution of features from weak to strong
*coupling, i.e., for the coupling parameter λ**A/B**/t* 1, using
many-body theory. First, we decouple the Fermionic and
Bosonic degrees of freedom near the vibrational impurity using
the small polaron transformation,^{26} that is, constructing the
Hamiltonian *H = e*^{S}*H e** ^{−S}*with

*S= i* *P*
*ω*_{0}

*mσ*

_{mσ}^{†}**λ(r***m**)**mσ**, P* *= (−i)(B − B*^{†}*).* (12)

We can write the resulting model according to
*H = −t*

*mnσ*

_{mσ}^{†}*e*^{−iλ(r}^{m}^{)P /ω}^{0}*σ*_{x}*e*^{i}^{λ(r}^{n}^{)P /ω}^{0}_{nσ}

*+ ω*0*B*^{†}*B*−

*mσ*

_{mσ}^{†}* λ(r*˜

*m*

*)*

*mσ*

_{2}

*,* (13)

where ˜**λ(r***m*)**= λ(r***m**)/*√
*ω*_{0}.

*The above expressions are valid for all couplings λ**A/B***(r***m*),
and clearly show that the presence of the inelastic scattering
center gives rise to an attractive interaction for the electrons
residing on the atoms surrounding the vibrational center. The
appearance of the electron-vibron couplings in the first term
of *H is due to the fact that S does not commute with a**iσ*^{†}*b**j σ*.

**A. Strong coupling limit**

Before we discuss the evolution of the electronic structure from the weak to strong coupling regime, we first consider a few observations about the strongly coupled system. In the

0.032 0.040 0.048

ωN(**r** **0****,**ω**)**
(a)

ω=15 meV

5 15 25

energy (meV) (b)

0.032 0.040 0.048

ωN(**r** **0****,**ω**)**

ω=15 meV (c)

0.032 0.040 0.048

ωN(**r** **0****,**ω**)**

ω=15 meV

**FIG. 2. (Color online) Change in the local IETS at r**_{0}in the weak
coupling limit for different asymmetric configurations with coupling
to (a) three, (b) two, and (c) one C atom in the nearest neighbor
hexagon, and distance from point of measurement, as indicated in
the upper insets. Left panels show the corresponding IETS maps at
*ω= ω*0. Parameters as in Fig.1(c).

strong coupling limit, the system reduces to a single impurity problem, with the difference to the conventional impurity problem being that here the impurity is constituted of up to six C atoms around the vibrational defect, depending on the symmetry/asymmetry of the coupling. For asymmetric coupling such that the vibrational impurity effectively couples to one C atom, the system reduces to a single site problem in which the Fermionic ground states can be written, for example,

*|2 = a*_{1↑}^{†}*a*_{1↓}* ^{†}* |, where | denotes the empty state, assuming

*that the vibrational impurity couples to atom n= 1 in the A*sublattice without loss of generality. The excited states are

*|σ = a*^{†}* _{1σ}*| and |0 = |, and the Fermionic energy spectrum

*can be written E*

*ν*

*= −(ν ˜λ*

*A1*)

^{2}

*, ν*

*= 0,1,2. The energy gain for*the doubly occupied site is evident from this result hence we

*expect this local attraction to play a major role in inducing*pairing correlations in graphene due to the local bosonic mode.

With the above observations in mind, we write the Hamil-
*tonian of the negative U site as*

*H*imp *= −˜λ*^{2}_{A1}

*σ*

(1*+ a*^{†}_{1 ¯}*σ**a*_{1 ¯}*σ**)a*_{1σ}^{†}*a*_{1σ}*.* (14)
*In terms of the eigenspectrum of the negative U center, we*
*write a*_{1σ}*= X*^{0σ}*+ σX*^{σ2}^{¯} *, where X*^{pq}*≡ |pq| denotes the*
transition from state*|q to |p and the factor σ ≡ σ**σ σ** ^{z}* . We can
thus write

*H*imp*= E*0*X*^{00}*+ E*1

*σ*

*X*^{σ σ}*+ E*2*X*^{22}*.* (15)

4 10 16

N(ω)

−0.6 0 0.6

energy (ω+3λ_{A1}^{2} )
(a)

2 5 8

N(ω)

(b)

−0.6 0 0.6

energy (ω+3λ_{A1}^{2} )

FIG. 3. DOS for the single site problem in the strong
*coupling/atomic limit using ω*0*= 15 meV and λ/D**c*= 2 × 10^{−2}
*for (a) T* *= 10 K and (b) T = 100 K.*

The spectrum of the single site is determined
through the GF ˜**G(t,t**^{})**= G***σ σ*^{}*(t,t*^{}**)F(t,t**^{}**), where G(t,t**^{})=
(−i)T*nσ**(t)*_{nσ}^{†}*(t*^{}) is the electronic GF and F*n**(t,t*^{})=
*{F**nαβ**(t,t*^{})}*α,β**=A,B*,

*F*_{nαβ}*(t,t*^{})*= X**nα**(t)X**nβ*^{†}*(t*^{})vib (16)
is the average over the bosonic degrees of freedom. Here

*X**nα**(t)= e*^{iω}^{0}^{B}^{†}^{Bt}*e*^{iλ}^{α}^{(r}^{n}^{)P /ω}^{0}*e*^{−iω}^{0}^{B}^{†}^{Bt}*,* *α= A,B. (17)*
Following the procedure lined out in Ref.27, we calculate the
*generalized function (τ* *= t − t*^{})

*F**nαβ**(t,t*^{})= exp

− 1

*2ω*^{2}_{0}[(1*+ 2n*0**)(λ***α***(r***n*)*+ λ**β***(r***n***))**^{2}

*− 2λ**α***(r***n**)λ**β***(r***n***)((1***+ n*0)(1*+ e** ^{−iωτ}*)

*+ n*0(1

*+ e*

^{iωτ}**))]**

*,* (18)

giving the Fourier-transformed GF
**G**˜^{r}_{σ σ}*(ω)= e*^{−(1+2n}^{0}^{)[λ}^{2}^{α}^{(r}^{n}^{)+λ}^{2}^{β}^{(r}^{n}^{)]/2ω}^{2}^{0}

×

*n*

*I**n*( ˜*ω*_{0}*)e*^{nβω}^{0}^{/2}**G**^{r}_{σ σ}*(ω− nω*0*),* (19)
where ˜*ω*_{0}*= 2λ**α***(r***n**)λ**β***(r***n*)√

*n*_{0}(1*+ n*0*)/ω*^{2}_{0}*and where I**n**(x) is*
the modified Bessel function. Thus for the single site problem
given by Eq.(14), the electronic ground state is in the atomic
limit given by the GF

*G*^{r}_{σ σ}*(ω)= δ**σ σ*

1*− a*_{1σ}^{†}*a*_{1σ}

*ω+ ˜λ*^{2}*Aa**+ iδ* + *a*_{1σ}^{†}*a*_{1σ}*ω+ 3˜λ*^{2}*Aa**+ iδ*

*,* (20)

*δ >*0. Setting*a*^{†}_{1σ}*a** _{1σ}* = 1, which corresponds to the double
occupied configuration, we reproduce the analogous spectrum
found in Ref.19for vibrational impurity on the surface of the
topological insulator, i.e., a series of sharp peaks centered
around the two-Fermion energy

*−3˜λ*

^{2}

*. This is shown in Fig. 3(a)*

_{A1}*for T*= 10 K and Fig. 3(b)

*for T*= 100 K, also showing that more inelastic side peaks become activated with increasing temperature, as expected. Similar conclusions

*hold for all our considered cases with N*

*= 1, . . . ,6 C atoms*coupling to the vibrational impurity, with the Fermionic

*ground state consisting of 2N electrons.*

**B. Evolution from weak to strong coupling**

Considering further the single site problem, now in the presence of the surrounding lattice, we write the transformed

lattice Hamiltonian as

*H*0*= H*0+ *H**T**,* (21)
*where the coupling between the negative U center and the*
lattice is given by

*H**T* =

**kσ**

*t*** _{k}**(1

*− e*

^{−iλ}

^{A1}

^{P /ω}^{0}

*)(X*

^{σ0}*+ σX*

^{2 ¯}

^{σ}*)b*

**kσ***+ H.c., (22)*with

*t*

**k**

*= −t*3

*n*=1*e*^{ik}^{·(r}^{1}^{+δ}^{n}^{)}*/*√

*N*, such that *t***k****±K** ≈

*±v**F**ke** ±i(π/3−ϕ)+ik·r*1

*/*√

*N. The negative U center hence*
couples to the surrounding lattice with an effective
*hybridization ˜t***k** *which is renormalized by the momentum P*
of the local bosonic mode.

We capture the evolution from the weak to strong coupling
limit by solving the equation of motion for the many-body
operator GF G_{a ¯}_{b}*(z)= X*^{a}*|X*^{b}^{¯}*(z), for the transitions a,b =*
*(0σ ),(σ 2) self-consistently in the mean-field approximation*
under the self-consistency condition that the occupation
*numbers N*0+

*σ**N**σ**+ N*2= 1. The occupation numbers
are calculated using^{28}

*N*_{0}= −1
*π*Im

*σ*

[1*− f (ω)]G*^{r}*0σ σ 0**(ω)dω,* (23a)
*N** _{σ}* = −1

*π*Im

*f(ω)G*^{r}_{0σ σ 0}*(ω)+ [1 − f (ω)]G*^{r}_{σ22σ}*(ω)*
*dω,*

(23b)
*N*_{2}= −1

*π*Im

*σ*

G^{r}_{σ22σ}*(ω)dω.* (23c)

Due to the inherent spin degeneracy and absence of a coupling
between the spin channels, the GF reduces to a 2× 2-matrix
*equation. To second order in t***k** *and ˜λ, the result is given in*
terms of the retarded GF

G^{r}*(ω) = (ω − − P(ω)(1 + σ*

*x*))

^{−1}

*P,*(24) where

*1*

**= diag{**_{2}

*},*

*n*

*= E*

*n*

*− E*

*n*−1, P

*= diag{P*1

*P*

_{2}},

*P*

_{1}

*= N*0

*+ N*1

*/2, P*

_{2}

*= N*1

*/2+ N*2

*, N*

_{1}=

*σ**N** _{σ}*, whereas

*the self-energy (ω)*=

*n**=1,2*^{(n)}*(ω) is given by*

^{(1)}*(ω)= −2ω*

1+

*ω*
*D**c*

2

2 log*D**c*

*|ω|+ iπsignω*

*,*

(25a)

^{(2)}*(ω)= −4πf(ω)*
*D*_{c}^{2}

*ω*
*ω*^{2}*− ω*_{0}^{2}

*ω+ ˜λ*^{2}

*ω+ ˜λ*^{2}*/2ω*^{3}*signω.* (25b)
*The contribution *^{(1)}accounts for fluctuations on and off the
*negative U center, essentially caused by the presence of the*
surrounding lattice, showing a cubic correction to the LDOS.

*The second contribution *^{(2)} is generated by fluctuations on
*and off the negative U center due to the coupling between the*
local vibrational mode and the Fermionic degrees of freedom.

Equation(24)using the self-energies in Eq.(25)should be solved self-consistently, however, we can make a few obser- vations on the expected behavior of the electronic structure.

*For weak coupling, the bare excitations E**ν**= −(ν ˜λ**A1*)^{2}→ 0.

*Thus for low energies such that ω/D**c* 1, we can neglect
*the self-energy *^{(2)} and approximate the first self-energy by

1 2 3 4

N(r1,ω) (x10−1)

10 22 30 40

0.2 0.6 1 1.4 1.8

N(r1,ω) (x10−1)

−800 −400 0 400 800 0.2

0.6 1 1.4 1.8

energy (meV) N(r1,ω) (x10−2)

−40 −20 0 20 40

1 2 3 4

energy (meV) N(r1,ω) (x10−3)

(a)

(c)

(b)

(d)

−800 −400 0 400 800 energy (meV)

0.2 1

1.8 x10^{3}

−2 −1 0 1 2

energy (eV)

FIG. 4. (Color online) Evolution of the LDOS at the negative
*Ucenter from weak to strong coupling regime. Here λ/D**c*= {5 ×
10^{−4}*,*1× 10^{−3}*,*5× 10^{−3}*,*1× 10^{−2}*}, ω*0*= 15 meV, and T = 10 K*
*(bold/black) and T* = 100 K (faint/red). The inset in panel (c) shows
*the full LDOS at T* = 100 K.

^{(1)}*≈ −2ω. Then the denominator of G** ^{r}*is given by

*3ω*

^{2}

*− 2ω*

2
*n*=1

* _{n}*+

2
*n*=1

_{n}*= 3(ω − *+*)(ω− *−*),* (26)
*where *_{±}= −(4 ∓√

*7)˜λ*^{2}*/3. This is found by observing that*

_{1}*= −˜λ*^{2} *and *2*= −3˜λ*^{2}, such that

*n**n**= −4˜λ*^{2} and

*n**n**= 3˜λ*^{4}*. Here we have, moreover, used that P*1*+ P*2=
*N*_{0}+

*σ**N**σ**+ N*2= 1 by charge conservation, along with
*P*_{n}*≈ 1/2, c.f. Fig.*5.

As the coupling is increased, the nonlinear components in the self-energies play an increasingly important role for the positions of the poles, such that we cannot any longer make use of Eq.(26).

In Figs.4(a)to4(d)we plot the evolution of the LDOS on
*the negative U center from weak to strong coupling regime for*
low (bold/black) and high (faint/red) temperatures. The LDOS
*ρ(ω)*= −tr ImG^{r}*(ω)/π is obtained from solving Eqs.* (23)
and(24)*self-consistently under the condition N*0+

*σ**N**σ*+
*N*_{2}= 1. In the weakly coupled system, panel 4 (a), there are
two main (elastic) peaks near the Fermi level, corresponding to

_{±}, c.f. Eq.(26). For low temperatures there is a tiny signature
*of a vibrational side peak at about ω= −ω*0= −15 meV. For
higher temperatures, these vibrational signatures become more
apparent, as one should expect since those modes are thermally
activated.

For increasing coupling the main elastic features remain, however, shifted to lower energies. They become increasingly broadened since the level width is a cubic function of the energy, c.f. Eq.(25a). Moreover, the presence of the vibrational side peaks also become more visible in the LDOS, even for low temperatures. In both cases illustrated by Figs.4(a)and4(b), the coupling is weak enough to preserve the overall Dirac cone, apart from the presence of the resonances.

For even stronger coupling, Figs.4(c)and4(d), the Dirac cone is fully destroyed and only the peak features, caused by the elastic and inelastic scattering, remain. Finally, in the strong coupling limit, Fig.4(d), there only appears a double peak structure, where the peaks correspond to the singly and

0.0002 0.001 0.005 0.2

0.5

occupation

λ/D_{c}
N_{2}
N0

N_{1}

*FIG. 5. (Color online) Evolution of the occupation numbers N*_{0}
*(triangles), N*1*(pentagrams), and N*2*(bullets), at the negative U center*
*from weak to strong coupling regime. Here ω*0*= 15 meV and T =*
10 K.

doubly occupied states. For high temperatures, the vibrational side peaks effectively act as a thermal broadening of the main peaks. The discrepancy with the situation illustrated in Fig.3 can be understood from the fact that we here take into account fluctuations to both the singly and doubly occupied states, hence there is a finite likelihood that even the singly occupied state becomes populated. This is a typical feature of any many- body description, and it emphasizes the fact that the charge is partially distributed among the available states.

We finally comment on the evolution of the Fermionic
*state of the negative U center from weak to strong coupling*
*regime, represented in terms of the populations numbers N**n*,
*n= 0,1,2, c.f. Fig.* 5. In the weakly coupled system, the
*energy of the single electron fluctuations **n**= −(n˜λ)*^{2}+
*(n*− 1)^{2}*˜λ*^{2}*= −(2n − 1)˜λ*^{2} lies below but close to the Fermi
level, c.f. Figs.4(a)and4(b), such that the system is open for
fluctuations between the (four) states. This property is verified
*by the occupation numbers, in that all N**n**, n= 0,1,2 are finite.*

This suggests the occurrence of local Cooper pair formation near the vibrational impurity, which will be the topic of a future publication.

In the strongly coupled limit, on the other hand, the set
of elastic and inelastic transition energies are far below the
Fermi level, c.f. Fig.4(d), such that the the population number
*N*_{0} *approaches zero. In other words, the negative U center*
acquires a Fermionic ground state which is a mixture of the
singly and doubly occupied states. The coupling between the
*negative U center and the surrounding lattice thus generates*
a more intricate electronic structure than what is suggested
*by the atomic limit physics where the negative U center is*
decoupled from the lattice.

In the intermediate regime, there is a cross-over regime,
or possibly a phase transition, c.f. crossing of population
*numbers near λ/D**c* 10^{−3} in Fig. 5, where the occupation
numbers of the empty and doubly occupied states evolve
monotonically decreasing and increasing, respectively, with
*the coupling strength λ, whereas the single Fermion state(s)*
remain constant.

It is finally worth mentioning that the attractive forces
indicated by Eq. (14) always have to be compared to the
repulsive Coulomb forces present in the material. For the case
of graphene, there is a controversy whether there is a significant
contribution to the electronic structure caused by the Coulomb
interaction, which is closely related to the question whether
the ground state of graphene is in a nonmagnetic semimetallic
state or an antiferromagnetic insulating state.^{29}While the latter
seems to be favorable for suspended graphene, the former

situation pertains to graphene deposited on a substrate which complies with our initial assumption. For this case, graphene is very well described by noninteracting electrons with negligible Coulomb interaction.

**V. CONCLUSION**

We have theoretically studied the effects of vibrational
impurity adsorbed onto graphene, specifically the inelastic
scattering properties. We find in the weak coupling regime
that the perturbed LDOS in the vicinity of the vibrational
impurity acquires peaks/dips and steps at the energy of the
vibrational mode. The spectral density distortions around
the vibrational mode is spatially extended showing inelastic
Friedel oscillations, in analogy with the findings for surfaces
of metallic materials^{23,25,30}and topological insulator.^{19}

By employing a many-body approach, we study the evolu-
tion from weak to strong coupling regime. In the weak coupling
regime, an elastic midgap resonance emerge, surrounded by
inelastic side resonances, at half the energy of the single
*electron fluctuations between the negative U center and the*
surrounding lattice. The finite occupation of all Fermionic
states, the empty, singly, and doubly occupied states, on
*the negative U site near the vibrational impurity in the*

weakly coupled system suggests local Cooper pair formation.

The aspects of this physics will be the topic of a future publication.

For intermediate coupling strength the peak structure is severely distorted and pushed below the Fermi level, leaving a strongly asymmetric Dirac cone around the Fermi level. The Dirac cone is eventually destroyed in the strongly coupled regime, in which the electronic structure acquires a band formed by the collection of elastic and inelastic resonances. We believe that our findings should be within the scope of present experimental local probing abilities using STM or atomic force microscopy.

**ACKNOWLEDGMENTS**

J.F. acknowledges B. Sanyal for communicating unpub- lished results and J.-X. Zhu for fruitful discussions. The authors thank the Swedish Research Council, EU, and Nordita for support. J.F. further acknowledges the Wenner-Gren Foundation for travel support. Work at LANL was carried out under the auspices of the US DOE under Contract No.

DE-AC52-06NA25396 through the Office of Basic Energy Sciences, Division of Materials Science and Engineering, and the UC Research Fee Program.

*Jonas.Fransson@physics.uu.se

1K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang,
S. V. Dubonos, I. V. Grigorieva, and A. A. Firsov,**Science 306, 666**
(2004).

2A. K. Geim and K. S. Novoselov, **Nat. Mater. 6, 183**
(2007).

3M. I. Katsnelson,**Mater. Today 10, 20 (2007).**

4A. H. Castro Neto, F. Guinea, N. M. R. Peres, K. S. Novoselov, and
A. K. Geim,**Rev. Mod. Phys. 81, 109 (2009).**

5M. A. H. Vozmediano, M. I. Katsnelson, and F. Guinea,Phys. Rep.

**496, 109 (2010).**

6D. C. Elias, R. R. Nair, T. M. G. Mohiuddin, S. V. Morozov, P. Blake,
M. P. Halsall, A. C. Ferrari, D. W. Boukhvalov, M. I. Katsnelson,
A. K. Geim, and K. S. Novoselov,**Science 323, 610 (2009).**

7S. H. M. Jafri, K. Carva, E. Widenkvist, T. Blom, B. Sanyal, J. Fransson, O. Eriksson, U. Jansson, H. Grennberg, O. Karis, R. A.

Quinlan, B. C. Holloway, and K. Leifer,**J. Phys. D 43, 045404**
(2010).

8K. Carva, B. Sanyal, J. Fransson, and O. Eriksson,**Phys. Rev. B 81,**
245405 (2010).

9T. O. Wehling, A. V. Balatsky, M. I. Katsnelson, A. I. Lichtenstein,
K. Scharnberg, and R. Wiesendanger,**Phys. Rev. B 75, 125425**
(2007).

10T. D. Stowe, K. Yasumura, T. W. Kenny, D. Botkin, K. Wago, and
D. Rugar,**Appl. Phys. Lett. 71, 288 (1997).**

11L. Gross, F. Mohn, P. Liljeroth, J. Repp, F. J. Giessibl, and G. Meyer,
**Science 324, 1428 (2009);**L. Gross, F. Mohn, N. Moll, P. Liljeroth,
and G. Meyer,**ibid. 325, 1110 (2009).**

12G. Binnig, H. Rohrer, Ch. Gerber, and E. Weibel,Phys. Rev. Lett.

**49, 57 (1982).**

13K. M. Lang, V. Madhavan, J. E. Hoffman, E. W. Hudson, H. Eisaki,
S. Uchida, and J. C. Davis,**Nature (London) 415, 412 (2002).**

14K. K. Gomes, A. N. Pasupathy, A. Pushp, S. Ono, Y. Ando, and
A. Yazdani,**Nature (London) 447, 569 (2007).**

15A. V. Balatsky, I. Vekhter, and J.-X. Zhu,**Rev. Mod. Phys. 78, 373**
(2006).

16Y. Hasegawa and Ph. Avouris,**Phys. Rev. Lett. 71, 1071 (1993).**

17M. F. Crommie, C. P. Lutz, and D. M. Eigler,**Nature (London) 363,**
524 (1993).

18M. Grobis, K. H. Khoo, R. Yamachika, X. Lu, K. Nagaoka, S. G.

Louie, M. F. Crommie, H. Kato, and H. Shinohara,Phys. Rev. Lett.

**94, 136802 (2005).**

19J.-H. She, J. Fransson, A. R. Bishop, and A. V. Balatsky,Phys. Rev.

**Lett. 110, 026802 (2013).**

20B. Sanyal, (unpublished).

21N. M. R. Peres, F. Guinea, and A. H. Castro Neto,**Phys. Rev. B 73,**
125411 (2006).

22E. Kogan, arXiv:1211.3369.

23J. Fransson and A. V. Balatsky,**Phys. Rev. B 75, 195337 (2007).**

24A. V. Balatsky, Ar. Abanov, and J.-X. Zhu,**Phys. Rev. B 68, 214506**
(2003).

25J. Fransson and A. V. Balatsky,**Phys. Rev. B 85, 161401(R) (2012).**

26**I. G. Lang and Y. A. Firsov, Zh. Eksp. Teor. Fiz. 43, 1843 (1962).**

27*G. D. Mahan, Many-Particle Physics (Plenum, New York, 1981).*

28J. Fransson,**Phys. Rev. B 72, 045415 (2005); 72, 075314 (2005);**

*Non-Equilibrium Nano-Physics (Springer, Dordrecht, 2010).*

29J. E. Drut and T. A. L¨ahde,**Phys. Rev. Lett. 102, 026802 (2009);**

**Phys. Rev. B 79, 165425 (2009).**

30H. Gawronski, J. Fransson, and K. Morgenstern, **Nano Lett. 11,**
2720 (2011).